#------------------------------------------------------------------------------
#$Date: 2021-06-09 11:34:31 +0300 (Wed, 09 Jun 2021) $
#$Revision: 266297 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/32/1563259.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1563259
loop_
_publ_author_name
'Guo, Li'
'Huang, Keke'
'Chen, Yan'
'Li, Guanghua'
'Yuan, Lin'
'Peng, Wen'
'Yuan, Hongming'
'Feng, Shouhua'
_publ_section_title
;
 Mild hydrothermal synthesis and ferrimagnetism of Pr3Fe5O12 and Nd3Fe5O12
 garnets
;
_journal_issue                   5
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              1048
_journal_page_last               1053
_journal_paper_doi               10.1016/j.jssc.2011.03.010
_journal_volume                  184
_journal_year                    2011
_chemical_formula_moiety         'Fe5 O12 Pr3'
_chemical_formula_sum            'Fe5 O12 Pr3'
_chemical_formula_weight         893.98
_space_group_IT_number           230
_space_group_name_Hall           '-I 4bd 2c 3'
_space_group_name_H-M_alt        'I a -3 d'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_H-M   'I a -3 d'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            8
_cell_length_a                   12.6695(15)
_cell_length_b                   12.6695(15)
_cell_length_c                   12.6695(15)
_cell_measurement_reflns_used    199
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.44
_cell_measurement_theta_min      3.94
_cell_volume                     2033.7(4)
_computing_cell_refinement       Process-auto
_computing_data_collection       Process-auto
_computing_data_reduction        Process-auto
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 10.0
_diffrn_measured_fraction_theta_full 0.990
_diffrn_measured_fraction_theta_max 0.990
_diffrn_measurement_device_type  'Rigaku RAXIS-RAPID'
_diffrn_measurement_method       omega-scan
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0358
_diffrn_reflns_av_sigmaI/netI    0.0116
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            8517
_diffrn_reflns_theta_full        27.44
_diffrn_reflns_theta_max         27.44
_diffrn_reflns_theta_min         3.94
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 0
_diffrn_standards_interval_time  0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    21.062
_exptl_absorpt_correction_type   none
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    5.840
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             3224
_exptl_crystal_size_max          0.18
_exptl_crystal_size_mid          0.18
_exptl_crystal_size_min          0.18
_refine_diff_density_max         0.554
_refine_diff_density_min         -1.419
_refine_diff_density_rms         0.220
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.292
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     17
_refine_ls_number_reflns         199
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.292
_refine_ls_R_factor_all          0.0233
_refine_ls_R_factor_gt           0.0220
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0186P)²+58.6657P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0568
_refine_ls_wR_factor_ref         0.0577
_reflns_number_gt                188
_reflns_number_total             199
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            JSSC-2011-184-1048.cif
_cod_data_source_block           Pr3Fe5O12
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_symmetry_cell_setting' value 'Cubic' was changed to
'cubic' in accordance with the built-in table derived from the CIF
Core dictionary named 'cif_core.dic' version 2.4.5 last updated on
2014-11-21.

data item '_exptl_crystal_density_meas' value 'none' was changed to
'?' -- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 8369 2020-08-20 11:38:08Z andrius 
;
_cod_original_sg_symbol_H-M      Ia-3d
_cod_database_code               1563259
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-x, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z'
'z, x, y'
'z+1/2, -x+1/2, -y'
'-z+1/2, -x, y+1/2'
'-z, x+1/2, -y+1/2'
'y, z, x'
'-y, z+1/2, -x+1/2'
'y+1/2, -z+1/2, -x'
'-y+1/2, -z, x+1/2'
'y+3/4, x+1/4, -z+1/4'
'-y+3/4, -x+3/4, -z+3/4'
'y+1/4, -x+1/4, z+3/4'
'-y+1/4, x+3/4, z+1/4'
'x+3/4, z+1/4, -y+1/4'
'-x+1/4, z+3/4, y+1/4'
'-x+3/4, -z+3/4, -y+3/4'
'x+1/4, -z+1/4, y+3/4'
'z+3/4, y+1/4, -x+1/4'
'z+1/4, -y+1/4, x+3/4'
'-z+1/4, y+3/4, x+1/4'
'-z+3/4, -y+3/4, -x+3/4'
'x+1/2, y+1/2, z+1/2'
'-x+1, -y+1/2, z+1'
'-x+1/2, y+1, -z+1'
'x+1, -y+1, -z+1/2'
'z+1/2, x+1/2, y+1/2'
'z+1, -x+1, -y+1/2'
'-z+1, -x+1/2, y+1'
'-z+1/2, x+1, -y+1'
'y+1/2, z+1/2, x+1/2'
'-y+1/2, z+1, -x+1'
'y+1, -z+1, -x+1/2'
'-y+1, -z+1/2, x+1'
'y+5/4, x+3/4, -z+3/4'
'-y+5/4, -x+5/4, -z+5/4'
'y+3/4, -x+3/4, z+5/4'
'-y+3/4, x+5/4, z+3/4'
'x+5/4, z+3/4, -y+3/4'
'-x+3/4, z+5/4, y+3/4'
'-x+5/4, -z+5/4, -y+5/4'
'x+3/4, -z+3/4, y+5/4'
'z+5/4, y+3/4, -x+3/4'
'z+3/4, -y+3/4, x+5/4'
'-z+3/4, y+5/4, x+3/4'
'-z+5/4, -y+5/4, -x+5/4'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'x, -y-1/2, z-1/2'
'-x-1/2, y-1/2, z'
'-z, -x, -y'
'-z-1/2, x-1/2, y'
'z-1/2, x, -y-1/2'
'z, -x-1/2, y-1/2'
'-y, -z, -x'
'y, -z-1/2, x-1/2'
'-y-1/2, z-1/2, x'
'y-1/2, z, -x-1/2'
'-y-3/4, -x-1/4, z-1/4'
'y-3/4, x-3/4, z-3/4'
'-y-1/4, x-1/4, -z-3/4'
'y-1/4, -x-3/4, -z-1/4'
'-x-3/4, -z-1/4, y-1/4'
'x-1/4, -z-3/4, -y-1/4'
'x-3/4, z-3/4, y-3/4'
'-x-1/4, z-1/4, -y-3/4'
'-z-3/4, -y-1/4, x-1/4'
'-z-1/4, y-1/4, -x-3/4'
'z-1/4, -y-3/4, -x-1/4'
'z-3/4, y-3/4, x-3/4'
'-x+1/2, -y+1/2, -z+1/2'
'x, y+1/2, -z'
'x+1/2, -y, z'
'-x, y, z+1/2'
'-z+1/2, -x+1/2, -y+1/2'
'-z, x, y+1/2'
'z, x+1/2, -y'
'z+1/2, -x, y'
'-y+1/2, -z+1/2, -x+1/2'
'y+1/2, -z, x'
'-y, z, x+1/2'
'y, z+1/2, -x'
'-y-1/4, -x+1/4, z+1/4'
'y-1/4, x-1/4, z-1/4'
'-y+1/4, x+1/4, -z-1/4'
'y+1/4, -x-1/4, -z+1/4'
'-x-1/4, -z+1/4, y+1/4'
'x+1/4, -z-1/4, -y+1/4'
'x-1/4, z-1/4, y-1/4'
'-x+1/4, z+1/4, -y-1/4'
'-z-1/4, -y+1/4, x+1/4'
'-z+1/4, y+1/4, -x-1/4'
'z+1/4, -y-1/4, -x+1/4'
'z-1/4, y-1/4, x-1/4'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Pr1 Pr 0.3750 0.5000 0.2500 0.0067(2) Uani 1 4 d S . .
Fe1 Fe 0.5000 0.5000 0.5000 0.0048(4) Uani 1 6 d S . .
Fe2 Fe 0.3750 0.5000 0.7500 0.0071(4) Uani 1 4 d S . .
O1 O 0.4701(3) 0.5528(3) 0.6488(3) 0.0051(7) Uani 1 1 d . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Pr Pr -0.2180 2.8214 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 Pr1 O1 111.07(17) 91 49_666
O1 Pr1 O1 72.76(17) 91 66_576
O1 Pr1 O1 159.53(17) 49_666 66_576
O1 Pr1 O1 159.53(17) 91 76_654
O1 Pr1 O1 72.76(17) 49_666 76_654
O1 Pr1 O1 111.07(17) 66_576 76_654
O1 Pr1 O1 124.81(8) 91 71_576
O1 Pr1 O1 95.49(10) 49_666 71_576
O1 Pr1 O1 67.68(16) 66_576 71_576
O1 Pr1 O1 73.34(13) 76_654 71_576
O1 Pr1 O1 95.49(10) 91 78_654
O1 Pr1 O1 124.81(8) 49_666 78_654
O1 Pr1 O1 73.34(13) 66_576 78_654
O1 Pr1 O1 67.68(16) 76_654 78_654
O1 Pr1 O1 107.85(17) 71_576 78_654
O1 Pr1 O1 67.68(16) 91 96
O1 Pr1 O1 73.34(13) 49_666 96
O1 Pr1 O1 124.81(8) 66_576 96
O1 Pr1 O1 95.49(10) 76_654 96
O1 Pr1 O1 166.37(16) 71_576 96
O1 Pr1 O1 73.84(16) 78_654 96
O1 Pr1 O1 73.34(13) 91 53_666
O1 Pr1 O1 67.68(16) 49_666 53_666
O1 Pr1 O1 95.49(10) 66_576 53_666
O1 Pr1 O1 124.81(8) 76_654 53_666
O1 Pr1 O1 73.84(16) 71_576 53_666
O1 Pr1 O1 166.37(16) 78_654 53_666
O1 Pr1 O1 107.85(17) 96 53_666
O1 Pr1 Fe2 36.38(9) 91 2_564
O1 Pr1 Fe2 143.62(9) 49_666 2_564
O1 Pr1 Fe2 36.38(9) 66_576 2_564
O1 Pr1 Fe2 143.62(9) 76_654 2_564
O1 Pr1 Fe2 96.81(8) 71_576 2_564
O1 Pr1 Fe2 83.19(8) 78_654 2_564
O1 Pr1 Fe2 96.81(8) 96 2_564
O1 Pr1 Fe2 83.19(8) 53_666 2_564
O1 Pr1 Fe2 143.62(9) 91 49_666
O1 Pr1 Fe2 36.38(9) 49_666 49_666
O1 Pr1 Fe2 143.62(9) 66_576 49_666
O1 Pr1 Fe2 36.38(9) 76_654 49_666
O1 Pr1 Fe2 83.19(8) 71_576 49_666
O1 Pr1 Fe2 96.81(8) 78_654 49_666
O1 Pr1 Fe2 83.19(8) 96 49_666
O1 Pr1 Fe2 96.81(8) 53_666 49_666
Fe2 Pr1 Fe2 180.0 2_564 49_666
O1 Pr1 Fe1 33.87(8) 91 14
O1 Pr1 Fe1 96.58(9) 49_666 14
O1 Pr1 Fe1 96.33(8) 66_576 14
O1 Pr1 Fe1 127.27(8) 76_654 14
O1 Pr1 Fe1 158.61(8) 71_576 14
O1 Pr1 Fe1 79.26(8) 78_654 14
O1 Pr1 Fe1 34.41(8) 96 14
O1 Pr1 Fe1 94.60(8) 53_666 14
Fe2 Pr1 Fe1 63.4 2_564 14
Fe2 Pr1 Fe1 116.6 49_666 14
O1 Pr1 Fe1 96.58(9) 91 .
O1 Pr1 Fe1 33.87(8) 49_666 .
O1 Pr1 Fe1 127.27(8) 66_576 .
O1 Pr1 Fe1 96.33(8) 76_654 .
O1 Pr1 Fe1 79.26(8) 71_576 .
O1 Pr1 Fe1 158.61(8) 78_654 .
O1 Pr1 Fe1 94.60(8) 96 .
O1 Pr1 Fe1 34.41(8) 53_666 .
Fe2 Pr1 Fe1 116.6 2_564 .
Fe2 Pr1 Fe1 63.4 49_666 .
Fe1 Pr1 Fe1 101.5 14 .
O1 Fe1 O1 180.0 57_666 9
O1 Fe1 O1 94.06(15) 57_666 .
O1 Fe1 O1 85.94(15) 9 .
O1 Fe1 O1 85.94(15) 57_666 53_666
O1 Fe1 O1 94.06(15) 9 53_666
O1 Fe1 O1 94.06(15) . 53_666
O1 Fe1 O1 94.06(15) 57_666 5
O1 Fe1 O1 85.94(15) 9 5
O1 Fe1 O1 85.94(15) . 5
O1 Fe1 O1 180.0 53_666 5
O1 Fe1 O1 85.94(15) 57_666 49_666
O1 Fe1 O1 94.06(15) 9 49_666
O1 Fe1 O1 180.00(7) . 49_666
O1 Fe1 O1 85.94(15) 53_666 49_666
O1 Fe1 O1 94.06(15) 5 49_666
O1 Fe1 Pr1 91.12(10) 57_666 .
O1 Fe1 Pr1 88.88(10) 9 .
O1 Fe1 Pr1 138.16(10) . .
O1 Fe1 Pr1 44.93(10) 53_666 .
O1 Fe1 Pr1 135.07(10) 5 .
O1 Fe1 Pr1 41.84(10) 49_666 .
O1 Fe1 Pr1 138.16(10) 57_666 57_666
O1 Fe1 Pr1 41.84(10) 9 57_666
O1 Fe1 Pr1 44.93(10) . 57_666
O1 Fe1 Pr1 88.88(10) 53_666 57_666
O1 Fe1 Pr1 91.12(10) 5 57_666
O1 Fe1 Pr1 135.07(10) 49_666 57_666
Pr1 Fe1 Pr1 113.6 . 57_666
O1 Fe1 Pr1 41.84(10) 57_666 9
O1 Fe1 Pr1 138.16(10) 9 9
O1 Fe1 Pr1 135.07(10) . 9
O1 Fe1 Pr1 91.12(10) 53_666 9
O1 Fe1 Pr1 88.88(10) 5 9
O1 Fe1 Pr1 44.93(10) 49_666 9
Pr1 Fe1 Pr1 66.4 . 9
Pr1 Fe1 Pr1 180.0 57_666 9
O1 Fe1 Pr1 135.07(10) 57_666 53_666
O1 Fe1 Pr1 44.93(10) 9 53_666
O1 Fe1 Pr1 91.12(10) . 53_666
O1 Fe1 Pr1 138.16(10) 53_666 53_666
O1 Fe1 Pr1 41.84(10) 5 53_666
O1 Fe1 Pr1 88.88(10) 49_666 53_666
Pr1 Fe1 Pr1 113.6 . 53_666
Pr1 Fe1 Pr1 66.4 57_666 53_666
Pr1 Fe1 Pr1 113.6 9 53_666
O1 Fe1 Pr1 44.93(10) 57_666 5
O1 Fe1 Pr1 135.07(10) 9 5
O1 Fe1 Pr1 88.88(10) . 5
O1 Fe1 Pr1 41.84(10) 53_666 5
O1 Fe1 Pr1 138.16(10) 5 5
O1 Fe1 Pr1 91.12(10) 49_666 5
Pr1 Fe1 Pr1 66.4 . 5
Pr1 Fe1 Pr1 113.6 57_666 5
Pr1 Fe1 Pr1 66.4 9 5
Pr1 Fe1 Pr1 180.0 53_666 5
O1 Fe1 Pr1 88.88(10) 57_666 49_666
O1 Fe1 Pr1 91.12(10) 9 49_666
O1 Fe1 Pr1 41.84(10) . 49_666
O1 Fe1 Pr1 135.07(10) 53_666 49_666
O1 Fe1 Pr1 44.93(10) 5 49_666
O1 Fe1 Pr1 138.16(10) 49_666 49_666
Pr1 Fe1 Pr1 180.0 . 49_666
Pr1 Fe1 Pr1 66.4 57_666 49_666
Pr1 Fe1 Pr1 113.6 9 49_666
Pr1 Fe1 Pr1 66.4 53_666 49_666
Pr1 Fe1 Pr1 113.6 5 49_666
O1 Fe2 O1 114.19(12) 68_657 28_456
O1 Fe2 O1 100.4(2) 68_657 89_665
O1 Fe2 O1 114.19(12) 28_456 89_665
O1 Fe2 O1 114.19(12) 68_657 .
O1 Fe2 O1 100.4(2) 28_456 .
O1 Fe2 O1 114.19(12) 89_665 .
O1 Fe2 Pr1 129.80(11) 68_657 49_666
O1 Fe2 Pr1 50.20(11) 28_456 49_666
O1 Fe2 Pr1 129.80(11) 89_665 49_666
O1 Fe2 Pr1 50.20(11) . 49_666
O1 Fe2 Pr1 50.20(11) 68_657 2_565
O1 Fe2 Pr1 129.80(11) 28_456 2_565
O1 Fe2 Pr1 50.20(11) 89_665 2_565
O1 Fe2 Pr1 129.80(11) . 2_565
Pr1 Fe2 Pr1 180.0 49_666 2_565
Fe2 O1 Fe1 129.26(19) . .
Fe2 O1 Pr1 93.42(14) . 49_666
Fe1 O1 Pr1 104.29(15) . 49_666
Fe2 O1 Pr1 121.68(17) . 57_666
Fe1 O1 Pr1 100.66(14) . 57_666
Pr1 O1 Pr1 102.24(13) 49_666 57_666
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Pr1 O1 2.438(4) 91
Pr1 O1 2.438(4) 49_666
Pr1 O1 2.438(4) 66_576
Pr1 O1 2.438(4) 76_654
Pr1 O1 2.545(4) 71_576
Pr1 O1 2.545(4) 78_654
Pr1 O1 2.545(4) 96
Pr1 O1 2.545(4) 53_666
Pr1 Fe2 3.1674(4) 2_564
Pr1 Fe2 3.1674(4) 49_666
Pr1 Fe1 3.5412(4) 14
Pr1 Fe1 3.5412(4) .
Fe1 O1 2.036(3) 57_666
Fe1 O1 2.036(3) 9
Fe1 O1 2.036(3) .
Fe1 O1 2.036(3) 53_666
Fe1 O1 2.036(3) 5
Fe1 O1 2.036(3) 49_666
Fe1 Pr1 3.5412(4) 57_666
Fe1 Pr1 3.5412(4) 9
Fe1 Pr1 3.5412(4) 53_666
Fe1 Pr1 3.5412(4) 5
Fe1 Pr1 3.5412(4) 49_666
Fe2 O1 1.882(4) 68_657
Fe2 O1 1.882(4) 28_456
Fe2 O1 1.882(4) 89_665
Fe2 O1 1.882(4) .
Fe2 Pr1 3.1674(4) 49_666
Fe2 Pr1 3.1674(4) 2_565
O1 Pr1 2.438(4) 49_666
O1 Pr1 2.545(4) 57_666
